#------------------------------------------------------------------------------
#$Date: 2017-08-31 06:27:55 +0300 (Thu, 31 Aug 2017) $
#$Revision: 200016 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/40/7044055.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7044055
loop_
_publ_author_name
'Kovrugin, Vadim M.'
'Colmont, Marie'
'Siidra, Oleg I.'
'Krivovichev, Sergey V.'
'Colis, Silviu'
'Mentré, Olivier'
_publ_section_title
;
 The First Lead Cobalt Phosphite, PbCo2(HPO3)3
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT02279D
_journal_year                    2017
_chemical_formula_moiety         'Co2 H3 O9 P3 Pb'
_chemical_formula_sum            'Co2 H3 O9 P3 Pb'
_chemical_formula_weight         564.98
_space_group_crystal_system      trigonal
_space_group_IT_number           160
_space_group_name_Hall           'R 3 -2"'
_space_group_name_H-M_alt        'R 3 m :H'
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.3145(15)
_cell_length_b                   5.3145(15)
_cell_length_c                   25.494(7)
_cell_measurement_reflns_used    3565
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      31.74
_cell_measurement_theta_min      2.40
_cell_volume                     623.6(3)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Crystal Maker (Crystal Maker, 2006)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 97)'
_computing_structure_solution    'Superflip (Palatinus & Chapuis, 2007)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0290
_diffrn_reflns_av_unetI/netI     0.0326
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            3590
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.973
_diffrn_reflns_theta_min         2.397
_exptl_absorpt_coefficient_mu    24.750
_exptl_absorpt_correction_T_max  0.7463
_exptl_absorpt_correction_T_min  0.6454
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    4.514
_exptl_crystal_description       'hexagonal prisms'
_exptl_crystal_F_000             768
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_refine_diff_density_max         1.485
_refine_diff_density_min         -0.555
_refine_diff_density_rms         0.128
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.062(12)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.034
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     41
_refine_ls_number_reflns         534
_refine_ls_number_restraints     4
_refine_ls_restrained_S_all      1.034
_refine_ls_R_factor_all          0.0147
_refine_ls_R_factor_gt           0.0147
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0063P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0298
_refine_ls_wR_factor_ref         0.0298
_reflns_Friedel_coverage         0.990
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                534
_reflns_number_total             534
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c7dt02279d1.cif
_cod_data_source_block           shelx
_cod_original_cell_volume        623.6(4)
_cod_database_code               7044055
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
'-y+1/3, -x+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Pb1 Pb 1.0000 1.0000 0.16209(2) 0.01761(10) Uani 1 6 d S T P
Co1 Co 1.0000 1.0000 0.28985(5) 0.0099(2) Uani 1 6 d S T P
Co2 Co 0.3333 0.6667 0.07026(5) 0.0096(3) Uani 1 6 d S T P
P1 P 0.6667 1.3333 0.09927(11) 0.0098(5) Uani 1 6 d DS T P
P2 P 1.6667 1.3333 0.32927(9) 0.0089(4) Uani 1 6 d DS T P
P3 P 0.3333 0.6667 0.25226(11) 0.0086(5) Uani 1 6 d DS T P
O1 O 1.3478(10) 1.1739(5) 0.34537(15) 0.0137(8) Uani 1 2 d S T P
O2 O 0.5100(5) 1.0199(9) 0.11827(17) 0.0185(9) Uani 1 2 d S T P
O3 O 0.6523(9) 0.8262(5) 0.23647(15) 0.0147(9) Uani 1 2 d S T P
H1 H 0.6667 1.3333 0.049(2) 0.022 Uiso 1 6 d DS U P
H2 H 1.6667 1.3333 0.273(3) 0.022 Uiso 1 6 d DS U P
H3 H 0.3333 0.6667 0.303(2) 0.022 Uiso 1 6 d DS U P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Pb1 O3 67.91(16) . 3_675
O3 Pb1 O3 67.91(16) . 2_765
O3 Pb1 O3 67.91(16) 3_675 2_765
O3 Pb1 O2 77.98(11) . .
O3 Pb1 O2 106.00(9) 3_675 .
O3 Pb1 O2 145.18(11) 2_765 .
O3 Pb1 O2 106.00(9) . 2_765
O3 Pb1 O2 145.18(11) 3_675 2_765
O3 Pb1 O2 77.98(11) 2_765 2_765
O2 Pb1 O2 105.95(9) . 2_765
O3 Pb1 O2 145.18(11) . 3_675
O3 Pb1 O2 77.98(11) 3_675 3_675
O3 Pb1 O2 106.00(9) 2_765 3_675
O2 Pb1 O2 105.95(9) . 3_675
O2 Pb1 O2 105.95(9) 2_765 3_675
O3 Pb1 O2 77.98(11) . 3_565
O3 Pb1 O2 145.18(11) 3_675 3_565
O3 Pb1 O2 106.00(9) 2_765 3_565
O2 Pb1 O2 58.45(17) . 3_565
O2 Pb1 O2 51.33(17) 2_765 3_565
O2 Pb1 O2 134.25(16) 3_675 3_565
O3 Pb1 O2 145.18(11) . 1_655
O3 Pb1 O2 106.00(9) 3_675 1_655
O3 Pb1 O2 77.98(11) 2_765 1_655
O2 Pb1 O2 134.25(16) . 1_655
O2 Pb1 O2 58.45(17) 2_765 1_655
O2 Pb1 O2 51.33(17) 3_675 1_655
O2 Pb1 O2 105.95(9) 3_565 1_655
O3 Pb1 O2 106.00(9) . 2_775
O3 Pb1 O2 77.98(11) 3_675 2_775
O3 Pb1 O2 145.18(11) 2_765 2_775
O2 Pb1 O2 51.33(17) . 2_775
O2 Pb1 O2 134.25(16) 2_765 2_775
O2 Pb1 O2 58.45(17) 3_675 2_775
O2 Pb1 O2 105.95(9) 3_565 2_775
O2 Pb1 O2 105.95(9) 1_655 2_775
O3 Pb1 Co1 40.16(10) . .
O3 Pb1 Co1 40.16(10) 3_675 .
O3 Pb1 Co1 40.16(10) 2_765 .
O2 Pb1 Co1 112.79(8) . .
O2 Pb1 Co1 112.80(8) 2_765 .
O2 Pb1 Co1 112.80(8) 3_675 .
O2 Pb1 Co1 112.80(8) 3_565 .
O2 Pb1 Co1 112.80(8) 1_655 .
O2 Pb1 Co1 112.80(8) 2_775 .
O3 Pb1 O1 118.85(13) . 13_444
O3 Pb1 O1 146.00(8) 3_675 13_444
O3 Pb1 O1 146.00(8) 2_765 13_444
O2 Pb1 O1 50.07(9) . 13_444
O2 Pb1 O1 68.09(8) 2_765 13_444
O2 Pb1 O1 85.97(10) 3_675 13_444
O2 Pb1 O1 50.07(9) 3_565 13_444
O2 Pb1 O1 85.97(10) 1_655 13_444
O2 Pb1 O1 68.09(8) 2_775 13_444
Co1 Pb1 O1 159.01(6) . 13_444
O3 Pb1 O1 146.00(8) . 15_674
O3 Pb1 O1 118.85(13) 3_675 15_674
O3 Pb1 O1 146.00(8) 2_765 15_674
O2 Pb1 O1 68.09(8) . 15_674
O2 Pb1 O1 85.97(10) 2_765 15_674
O2 Pb1 O1 50.07(9) 3_675 15_674
O2 Pb1 O1 85.97(10) 3_565 15_674
O2 Pb1 O1 68.09(8) 1_655 15_674
O2 Pb1 O1 50.07(9) 2_775 15_674
Co1 Pb1 O1 159.01(6) . 15_674
O1 Pb1 O1 36.14(10) 13_444 15_674
O3 Co1 O3 82.56(17) 2_765 3_675
O3 Co1 O3 82.56(17) 2_765 .
O3 Co1 O3 82.56(17) 3_675 .
O3 Co1 O1 98.26(11) 2_765 .
O3 Co1 O1 98.26(11) 3_675 .
O3 Co1 O1 178.89(17) . .
O3 Co1 O1 178.89(17) 2_765 2_765
O3 Co1 O1 98.27(11) 3_675 2_765
O3 Co1 O1 98.27(11) . 2_765
O1 Co1 O1 80.90(17) . 2_765
O3 Co1 O1 98.27(11) 2_765 3_675
O3 Co1 O1 178.89(17) 3_675 3_675
O3 Co1 O1 98.27(11) . 3_675
O1 Co1 O1 80.90(17) . 3_675
O1 Co1 O1 80.90(17) 2_765 3_675
O3 Co1 Co2 130.38(11) 2_765 7
O3 Co1 Co2 130.38(11) 3_675 7
O3 Co1 Co2 130.38(11) . 7
O1 Co1 Co2 48.52(11) . 7
O1 Co1 Co2 48.52(11) 2_765 7
O1 Co1 Co2 48.52(11) 3_675 7
O3 Co1 Pb1 49.62(11) 2_765 .
O3 Co1 Pb1 49.62(11) 3_675 .
O3 Co1 Pb1 49.62(11) . .
O1 Co1 Pb1 131.48(11) . .
O1 Co1 Pb1 131.48(11) 2_765 .
O1 Co1 Pb1 131.48(11) 3_675 .
Co2 Co1 Pb1 180.0 7 .
O2 Co2 O2 87.57(17) 2_665 3_565
O2 Co2 O2 87.57(17) 2_665 .
O2 Co2 O2 87.57(17) 3_565 .
O2 Co2 O1 96.66(12) 2_665 14_654
O2 Co2 O1 174.13(17) 3_565 14_654
O2 Co2 O1 96.66(12) . 14_654
O2 Co2 O1 96.66(12) 2_665 15_564
O2 Co2 O1 96.66(12) 3_565 15_564
O2 Co2 O1 174.13(17) . 15_564
O1 Co2 O1 78.85(17) 14_654 15_564
O2 Co2 O1 174.13(17) 2_665 13_444
O2 Co2 O1 96.66(12) 3_565 13_444
O2 Co2 O1 96.66(12) . 13_444
O1 Co2 O1 78.85(17) 14_654 13_444
O1 Co2 O1 78.85(17) 15_564 13_444
O2 Co2 Co1 126.97(12) 2_665 13_444
O2 Co2 Co1 126.97(12) 3_565 13_444
O2 Co2 Co1 126.97(12) . 13_444
O1 Co2 Co1 47.16(11) 14_654 13_444
O1 Co2 Co1 47.16(11) 15_564 13_444
O1 Co2 Co1 47.16(11) 13_444 13_444
O2 P1 O2 110.37(19) 2_775 3_575
O2 P1 O2 110.37(19) 2_775 .
O2 P1 O2 110.37(19) 3_575 .
O2 P1 O1 147.44(17) 2_775 15_574
O2 P1 O1 65.41(17) 3_575 15_574
O2 P1 O1 100.72(14) . 15_574
O2 P1 O1 100.71(14) 2_775 13_454
O2 P1 O1 65.41(17) 3_575 13_454
O2 P1 O1 147.44(17) . 13_454
O1 P1 O1 47.16(14) 15_574 13_454
O2 P1 O1 147.44(17) 2_775 14_654
O2 P1 O1 100.72(14) 3_575 14_654
O2 P1 O1 65.41(17) . 14_654
O1 P1 O1 43.02(14) 15_574 14_654
O1 P1 O1 83.25(9) 13_454 14_654
O2 P1 O1 65.41(17) 2_775 14_764
O2 P1 O1 100.72(14) 3_575 14_764
O2 P1 O1 147.44(17) . 14_764
O1 P1 O1 83.25(9) 15_574 14_764
O1 P1 O1 43.02(14) 13_454 14_764
O1 P1 O1 100.12(12) 14_654 14_764
O2 P1 O1 100.72(14) 2_775 13_444
O2 P1 O1 147.44(17) 3_575 13_444
O2 P1 O1 65.41(17) . 13_444
O1 P1 O1 83.24(9) 15_574 13_444
O1 P1 O1 100.12(12) 13_454 13_444
O1 P1 O1 47.16(14) 14_654 13_444
O1 P1 O1 83.24(9) 14_764 13_444
O2 P1 O1 65.41(17) 2_775 15_674
O2 P1 O1 147.44(17) 3_575 15_674
O2 P1 O1 100.72(14) . 15_674
O1 P1 O1 100.12(12) 15_574 15_674
O1 P1 O1 83.24(9) 13_454 15_674
O1 P1 O1 83.24(9) 14_654 15_674
O1 P1 O1 47.16(14) 14_764 15_674
O1 P1 O1 43.02(14) 13_444 15_674
O1 P2 O1 113.02(14) . 2_865
O1 P2 O1 113.02(14) . 3_785
O1 P2 O1 113.02(14) 2_865 3_785
O1 P2 O3 64.23(15) . 2_765
O1 P2 O3 99.28(13) 2_865 2_765
O1 P2 O3 144.18(15) 3_785 2_765
O1 P2 O3 99.28(13) . 1_655
O1 P2 O3 64.23(15) 2_865 1_655
O1 P2 O3 144.18(15) 3_785 1_655
O3 P2 O3 41.87(14) 2_765 1_655
O1 P2 O3 144.18(15) . 3_775
O1 P2 O3 64.23(15) 2_865 3_775
O1 P2 O3 99.28(13) 3_785 3_775
O3 P2 O3 80.62(8) 2_765 3_775
O3 P2 O3 45.84(14) 1_655 3_775
O1 P2 O3 144.18(15) . 2_875
O1 P2 O3 99.28(13) 2_865 2_875
O1 P2 O3 64.23(15) 3_785 2_875
O3 P2 O3 96.62(11) 2_765 2_875
O3 P2 O3 80.62(8) 1_655 2_875
O3 P2 O3 41.87(14) 3_775 2_875
O1 P2 O3 64.23(15) . 3_675
O1 P2 O3 144.18(15) 2_865 3_675
O1 P2 O3 99.28(13) 3_785 3_675
O3 P2 O3 45.84(14) 2_765 3_675
O3 P2 O3 80.62(8) 1_655 3_675
O3 P2 O3 96.62(11) 3_775 3_675
O3 P2 O3 80.62(8) 2_875 3_675
O1 P2 O3 99.28(13) . 1_665
O1 P2 O3 144.18(15) 2_865 1_665
O1 P2 O3 64.23(15) 3_785 1_665
O3 P2 O3 80.62(8) 2_765 1_665
O3 P2 O3 96.62(11) 1_655 1_665
O3 P2 O3 80.62(8) 3_775 1_665
O3 P2 O3 45.84(14) 2_875 1_665
O3 P2 O3 41.87(14) 3_675 1_665
O3 P3 O3 113.27(14) 2_665 3_565
O3 P3 O3 113.27(14) 2_665 .
O3 P3 O3 113.27(14) 3_565 .
O3 P3 O1 99.09(13) 2_665 2_765
O3 P3 O1 143.89(16) 3_565 2_765
O3 P3 O1 64.05(15) . 2_765
O3 P3 O1 64.05(15) 2_665 1_455
O3 P3 O1 143.89(16) 3_565 1_455
O3 P3 O1 99.09(13) . 1_455
O1 P3 O1 41.78(14) 2_765 1_455
O3 P3 O1 64.05(15) 2_665 3_575
O3 P3 O1 99.09(13) 3_565 3_575
O3 P3 O1 143.89(16) . 3_575
O1 P3 O1 80.47(9) 2_765 3_575
O1 P3 O1 45.79(14) 1_455 3_575
O3 P3 O1 99.09(13) 2_665 2_655
O3 P3 O1 64.05(15) 3_565 2_655
O3 P3 O1 143.89(16) . 2_655
O1 P3 O1 96.43(11) 2_765 2_655
O1 P3 O1 80.47(9) 1_455 2_655
O1 P3 O1 41.78(14) 3_575 2_655
O3 P3 O1 143.89(16) 2_665 3_675
O3 P3 O1 99.09(13) 3_565 3_675
O3 P3 O1 64.05(15) . 3_675
O1 P3 O1 45.79(14) 2_765 3_675
O1 P3 O1 80.47(9) 1_455 3_675
O1 P3 O1 96.43(11) 3_575 3_675
O1 P3 O1 80.47(9) 2_655 3_675
O3 P3 O1 143.89(16) 2_665 1_445
O3 P3 O1 64.05(15) 3_565 1_445
O3 P3 O1 99.09(13) . 1_445
O1 P3 O1 80.47(9) 2_765 1_445
O1 P3 O1 96.43(11) 1_455 1_445
O1 P3 O1 80.47(9) 3_575 1_445
O1 P3 O1 45.79(14) 2_655 1_445
O1 P3 O1 41.78(14) 3_675 1_445
P2 O1 Co1 122.9(2) . .
P2 O1 Co2 152.8(3) . 7
Co1 O1 Co2 84.32(16) . 7
P2 O1 O1 33.49(7) . 3_785
Co1 O1 O1 130.45(8) . 3_785
Co2 O1 O1 129.42(8) 7 3_785
P2 O1 O1 33.49(7) . 2_865
Co1 O1 O1 130.45(8) . 2_865
Co2 O1 O1 129.42(8) 7 2_865
O1 O1 O1 60.0 3_785 2_865
P2 O1 O1 146.51(7) . 3_675
Co1 O1 O1 49.55(8) . 3_675
Co2 O1 O1 50.58(8) 7 3_675
O1 O1 O1 180.0 3_785 3_675
O1 O1 O1 120.000(1) 2_865 3_675
P2 O1 O1 146.51(7) . 2_765
Co1 O1 O1 49.55(8) . 2_765
Co2 O1 O1 50.58(8) 7 2_765
O1 O1 O1 120.000(1) 3_785 2_765
O1 O1 O1 180.00(18) 2_865 2_765
O1 O1 O1 60.0 3_675 2_765
P2 O1 O2 118.2(2) . 9_565
Co1 O1 O2 112.44(15) . 9_565
Co2 O1 O2 39.88(9) 7 9_565
O1 O1 O2 116.09(8) 3_785 9_565
O1 O1 O2 89.61(10) 2_865 9_565
O1 O1 O2 63.91(8) 3_675 9_565
O1 O1 O2 90.39(10) 2_765 9_565
P2 O1 O2 118.2(2) . 7
Co1 O1 O2 112.44(15) . 7
Co2 O1 O2 39.88(9) 7 7
O1 O1 O2 89.61(10) 3_785 7
O1 O1 O2 116.09(8) 2_865 7
O1 O1 O2 90.39(10) 3_675 7
O1 O1 O2 63.91(8) 2_765 7
O2 O1 O2 53.06(16) 9_565 7
P2 O1 O3 90.41(17) . 2_765
Co1 O1 O3 40.44(9) . 2_765
Co2 O1 O3 113.94(16) 7 2_765
O1 O1 O3 115.64(8) 3_785 2_765
O1 O1 O3 90.01(11) 2_865 2_765
O1 O1 O3 64.37(8) 3_675 2_765
O1 O1 O3 89.99(11) 2_765 2_765
O2 O1 O3 119.25(9) 9_565 2_765
O2 O1 O3 151.04(18) 7 2_765
P2 O1 O3 90.41(17) . 3_675
Co1 O1 O3 40.44(9) . 3_675
Co2 O1 O3 113.94(16) 7 3_675
O1 O1 O3 90.01(11) 3_785 3_675
O1 O1 O3 115.64(8) 2_865 3_675
O1 O1 O3 89.99(11) 3_675 3_675
O1 O1 O3 64.37(8) 2_765 3_675
O2 O1 O3 151.04(18) 9_565 3_675
O2 O1 O3 119.25(9) 7 3_675
O3 O1 O3 51.25(16) 2_765 3_675
P2 O1 P1 101.04(14) . 7_545
Co1 O1 P1 114.24(11) . 7_545
Co2 O1 P1 63.23(7) 7 7_545
O1 O1 P1 113.58(7) 3_785 7_545
O1 O1 P1 68.49(7) 2_865 7_545
O1 O1 P1 66.42(7) 3_675 7_545
O1 O1 P1 111.51(7) 2_765 7_545
O2 O1 P1 26.03(8) 9_565 7_545
O2 O1 P1 77.67(11) 7 7_545
O3 O1 P1 102.68(8) 2_765 7_545
O3 O1 P1 151.97(14) 3_675 7_545
P1 O2 Co2 124.5(3) . .
P1 O2 O2 34.81(9) . 3_575
Co2 O2 O2 133.78(9) . 3_575
P1 O2 O2 34.81(9) . 2_775
Co2 O2 O2 133.78(9) . 2_775
O2 O2 O2 60.0 3_575 2_775
P1 O2 O2 145.18(9) . 2_665
Co2 O2 O2 46.22(9) . 2_665
O2 O2 O2 119.999(1) 3_575 2_665
O2 O2 O2 180.0 2_775 2_665
P1 O2 O2 145.18(9) . 3_565
Co2 O2 O2 46.22(9) . 3_565
O2 O2 O2 180.0 3_575 3_565
O2 O2 O2 120.0 2_775 3_565
O2 O2 O2 60.0 2_665 3_565
P1 O2 Pb1 98.83(11) . .
Co2 O2 Pb1 101.98(10) . .
O2 O2 Pb1 119.22(8) 3_575 .
O2 O2 Pb1 64.33(8) 2_775 .
O2 O2 Pb1 115.67(8) 2_665 .
O2 O2 Pb1 60.78(8) 3_565 .
P1 O2 Pb1 98.83(11) . 1_455
Co2 O2 Pb1 101.98(10) . 1_455
O2 O2 Pb1 64.33(8) 3_575 1_455
O2 O2 Pb1 119.22(8) 2_775 1_455
O2 O2 Pb1 60.78(8) 2_665 1_455
O2 O2 Pb1 115.67(8) 3_565 1_455
Pb1 O2 Pb1 134.25(16) . 1_455
P1 O2 O1 88.56(19) . 14_654
Co2 O2 O1 43.46(10) . 14_654
O2 O2 O1 90.39(10) 3_575 14_654
O2 O2 O1 116.53(8) 2_775 14_654
O2 O2 O1 63.47(8) 2_665 14_654
O2 O2 O1 89.61(10) 3_565 14_654
Pb1 O2 O1 136.86(14) . 14_654
Pb1 O2 O1 85.37(8) 1_455 14_654
P1 O2 O1 88.56(19) . 13_444
Co2 O2 O1 43.46(10) . 13_444
O2 O2 O1 116.53(8) 3_575 13_444
O2 O2 O1 90.39(10) 2_775 13_444
O2 O2 O1 89.61(10) 2_665 13_444
O2 O2 O1 63.47(8) 3_565 13_444
Pb1 O2 O1 85.37(8) . 13_444
Pb1 O2 O1 136.86(14) 1_455 13_444
O1 O2 O1 52.18(16) 14_654 13_444
P1 O2 O3 122.2(2) . .
Co2 O2 O3 108.93(16) . .
O2 O2 O3 114.54(7) 3_575 .
O2 O2 O3 92.31(9) 2_775 .
O2 O2 O3 87.69(9) 2_665 .
O2 O2 O3 65.46(7) 3_565 .
Pb1 O2 O3 45.71(9) . .
Pb1 O2 O3 89.59(13) 1_455 .
O1 O2 O3 149.28(17) 14_654 .
O1 O2 O3 121.99(10) 13_444 .
P1 O2 O3 122.2(2) . 2_665
Co2 O2 O3 108.93(16) . 2_665
O2 O2 O3 92.31(9) 3_575 2_665
O2 O2 O3 114.54(7) 2_775 2_665
O2 O2 O3 65.46(7) 2_665 2_665
O2 O2 O3 87.69(9) 3_565 2_665
Pb1 O2 O3 89.59(13) . 2_665
Pb1 O2 O3 45.71(9) 1_455 2_665
O1 O2 O3 121.99(10) 14_654 2_665
O1 O2 O3 149.28(17) 13_444 2_665
O3 O2 O3 44.05(15) . 2_665
P3 O3 Co1 124.3(2) . .
P3 O3 Pb1 145.5(2) . .
Co1 O3 Pb1 90.21(16) . .
P3 O3 O3 33.36(7) . 3_565
Co1 O3 O3 131.28(8) . 3_565
Pb1 O3 O3 123.96(8) . 3_565
P3 O3 O3 33.36(7) . 2_665
Co1 O3 O3 131.28(8) . 2_665
Pb1 O3 O3 123.96(8) . 2_665
O3 O3 O3 60.0 3_565 2_665
P3 O3 O3 146.64(7) . 3_675
Co1 O3 O3 48.72(8) . 3_675
Pb1 O3 O3 56.05(8) . 3_675
O3 O3 O3 180.0 3_565 3_675
O3 O3 O3 120.0 2_665 3_675
P3 O3 O3 146.64(7) . 2_765
Co1 O3 O3 48.72(8) . 2_765
Pb1 O3 O3 56.05(8) . 2_765
O3 O3 O3 120.0 3_565 2_765
O3 O3 O3 180.00(9) 2_665 2_765
O3 O3 O3 60.0 3_675 2_765
P3 O3 O1 90.66(18) . 2_765
Co1 O3 O1 41.29(9) . 2_765
Pb1 O3 O1 120.07(15) . 2_765
O3 O3 O1 115.62(8) 3_565 2_765
O3 O3 O1 89.99(11) 2_665 2_765
O3 O3 O1 64.38(8) 3_675 2_765
O3 O3 O1 90.01(11) 2_765 2_765
P3 O3 O1 90.66(18) . 3_675
Co1 O3 O1 41.29(9) . 3_675
Pb1 O3 O1 120.07(15) . 3_675
O3 O3 O1 89.99(11) 3_565 3_675
O3 O3 O1 115.62(8) 2_665 3_675
O3 O3 O1 90.01(11) 3_675 3_675
O3 O3 O1 64.38(8) 2_765 3_675
O1 O3 O1 51.27(16) 2_765 3_675
P3 O3 O2 92.79(18) . .
Co1 O3 O2 136.31(16) . .
Pb1 O3 O2 56.31(8) . .
O3 O3 O2 92.31(9) 3_565 .
O3 O3 O2 67.97(7) 2_665 .
O3 O3 O2 87.69(9) 3_675 .
O3 O3 O2 112.03(7) 2_765 .
O1 O3 O2 129.69(10) 2_765 .
O1 O3 O2 176.39(15) 3_675 .
P3 O3 O2 92.79(18) . 3_565
Co1 O3 O2 136.31(16) . 3_565
Pb1 O3 O2 56.31(8) . 3_565
O3 O3 O2 67.97(7) 3_565 3_565
O3 O3 O2 92.31(9) 2_665 3_565
O3 O3 O2 112.03(7) 3_675 3_565
O3 O3 O2 87.69(9) 2_765 3_565
O1 O3 O2 176.39(15) 2_765 3_565
O1 O3 O2 129.69(10) 3_675 3_565
O2 O3 O2 49.08(15) . 3_565
P3 O3 P2 80.91(12) . 1_445
Co1 O3 P2 63.59(7) . 1_445
Pb1 O3 P2 119.74(9) . 1_445
O3 O3 P2 69.06(7) 3_565 1_445
O3 O3 P2 112.92(7) 2_665 1_445
O3 O3 P2 110.93(7) 3_675 1_445
O3 O3 P2 67.08(7) 2_765 1_445
O1 O3 P2 75.08(11) 2_765 1_445
O1 O3 P2 25.35(8) 3_675 1_445
O2 O3 P2 154.79(12) . 1_445
O2 O3 P2 106.52(7) 3_565 1_445
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pb1 O3 2.481(4) .
Pb1 O3 2.481(4) 3_675
Pb1 O3 2.481(4) 2_765
Pb1 O2 2.8841(18) .
Pb1 O2 2.8841(18) 2_765
Pb1 O2 2.8841(18) 3_675
Pb1 O2 2.8841(18) 3_565
Pb1 O2 2.8841(18) 1_655
Pb1 O2 2.8841(18) 2_775
Pb1 Co1 3.2569(16) .
Pb1 O1 4.097(4) 13_444
Pb1 O1 4.097(4) 15_674
Co1 O3 2.101(4) 2_765
Co1 O3 2.101(4) 3_675
Co1 O3 2.101(4) .
Co1 O1 2.137(4) .
Co1 O1 2.137(4) 2_765
Co1 O1 2.137(4) 3_675
Co1 Co2 2.9000(19) 7
Co2 O2 2.035(4) 2_665
Co2 O2 2.035(4) 3_565
Co2 O2 2.035(4) .
Co2 O1 2.183(4) 14_654
Co2 O1 2.183(4) 15_564
Co2 O1 2.183(4) 13_444
Co2 Co1 2.9000(19) 13_444
P1 O2 1.522(4) 2_775
P1 O2 1.522(4) 3_575
P1 O2 1.522(4) .
P1 O1 3.466(3) 15_574
P1 O1 3.466(3) 13_454
P1 O1 3.466(3) 14_654
P1 O1 3.466(3) 14_764
P1 O1 3.466(3) 13_444
P1 O1 3.466(3) 15_674
P2 O1 1.524(4) .
P2 O1 1.524(4) 2_865
P2 O1 1.524(4) 3_785
P2 O3 3.558(3) 2_765
P2 O3 3.558(3) 1_655
P2 O3 3.558(3) 3_775
P2 O3 3.558(3) 2_875
P2 O3 3.558(3) 3_675
P2 O3 3.558(3) 1_665
P3 O3 1.522(4) 2_665
P3 O3 1.522(4) 3_565
P3 O3 1.522(4) .
P3 O1 3.564(3) 2_765
P3 O1 3.564(3) 1_455
P3 O1 3.564(3) 3_575
P3 O1 3.564(3) 2_655
P3 O1 3.564(3) 3_675
P3 O1 3.564(3) 1_445
O1 Co2 2.183(4) 7
O1 O1 2.542(8) 3_785
O1 O1 2.542(8) 2_865
O1 O1 2.773(8) 3_675
O1 O1 2.773(8) 2_765
O1 O2 3.152(5) 9_565
O1 O2 3.152(5) 7
O1 O3 3.205(5) 2_765
O1 O3 3.205(5) 3_675
O1 P1 3.466(3) 7_545
O2 O2 2.498(7) 3_575
O2 O2 2.498(7) 2_775
O2 O2 2.816(7) 2_665
O2 O2 2.816(7) 3_565
O2 Pb1 2.8841(18) 1_455
O2 O1 3.152(5) 14_654
O2 O1 3.152(5) 13_444
O2 O3 3.390(5) .
O2 O3 3.390(5) 2_665
O3 O3 2.543(8) 3_565
O3 O3 2.543(8) 2_665
O3 O3 2.772(8) 3_675
O3 O3 2.772(8) 2_765
O3 O1 3.205(5) 2_765
O3 O1 3.205(5) 3_675
O3 O2 3.390(5) 3_565
O3 P2 3.558(3) 1_445
